Heterobimetallic hexanuclear [Mn(ΙΙΙ)(4)Ln(ΙΙΙ)(2)] clusters: A rare Mn(ΙΙΙ)(4)Nd(ΙΙΙ)(2) example exhibiting slow relaxation of magnetization.
Ke, Hongshan; Zhao, Lang; Guo, Yang; Tang, Jinkui; Dalton transactions (Cambridge, England : 2003) 41 (2012) 2314–2319; doi:10.1039/c2dt11922f

data_7018056
_publ_section_title
;
 Heterobimetallic hexanuclear [Mn(\I\I\I)(4)Ln(\I\I\I)(2)] clusters: A
 rare Mn(\I\I\I)(4)Nd(\I\I\I)(2) example exhibiting slow relaxation of
 magnetization.
;
_journal_issue                   8
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              2314
_journal_page_last               2319
_journal_paper_doi               10.1039/c2dt11922f
_journal_volume                  41
_journal_year                    2012
_chemical_formula_sum            'C68 H116 Cl2 La2 Mn4 N4 O48'
_chemical_formula_weight         2326.13
_chemical_name_systematic
;
?
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 106.2960(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   13.3143(7)
_cell_length_b                   22.1979(11)
_cell_length_c                   16.4153(7)
_cell_measurement_temperature    176(2)
_cell_volume                     4656.6(4)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      176(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0409
_diffrn_reflns_av_sigmaI/netI    0.0428
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       27
_diffrn_reflns_limit_k_min       -27
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            30473
_diffrn_reflns_theta_full        26.02
_diffrn_reflns_theta_max         26.02
_diffrn_reflns_theta_min         1.58
_exptl_absorpt_coefficient_mu    1.577
_exptl_absorpt_correction_T_max  0.7432
_exptl_absorpt_correction_T_min  0.6938
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            Black
_exptl_crystal_density_diffrn    1.659
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Block
_exptl_crystal_F_000             2368
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.23
_exptl_crystal_size_min          0.20
_refine_diff_density_max         1.893
_refine_diff_density_min         -0.790
_refine_diff_density_rms         0.195
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.071
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     598
_refine_ls_number_reflns         9156
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.071
_refine_ls_R_factor_all          0.0517
_refine_ls_R_factor_gt           0.0381
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0589P)^2^+5.6739P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1003
_refine_ls_wR_factor_ref         0.1127
_reflns_number_gt                7456
_reflns_number_total             9156
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c2dt11922f.txt
_cod_data_source_block           1
_cod_original_sg_symbol_H-M      P2(1)/c
_cod_database_code               7018056